This is a repository copy of
Novel Metal Silicide Thin Films by Design via Controlled
White Rose Research Online URL for this paper:
Version: Accepted Version
Streller, F, Agarwal, R, Mangolini, F et al. (1 more author) (2015) Novel Metal Silicide Thin
Films by Design via Controlled Solid-State Diffusion. Chemistry of Materials, 27 (12). 4247
- 4253. ISSN 0897-4756
If you consider content in White Rose Research Online to be in breach of UK law, please notify us by
and Robert W. Carpick*, ,à
Department of Materials Science and Engineering, University of Pennsylvania, 3231 Walnut Street, Philadelphia, Pennsylvania 19104, United States
Department of Mechanical Engineering and Applied Mechanics, University of Pennsylvania, 220 S. 33rd Street, Phil-adelphia, Pennsylvania 19104, United States
: In the quest to accelerate the discovery and deployment of new materials with ideal and tailored properties, synthesis via solid-state diffusion holds particular promise as it allows the crystal structure and stoichiometry of thin films to be controlled independently of the deposition method. However, the kinetics and the quality of the resulting materials re-main relatively unexplored. Here we demonstrate both source-limited and kinetically-limited solid-state diffusion as novel routes to tune the stoichiometry of platinum silicide (PtxSi) thin films, representative of metal silicides which have attractive mechanical and electronic properties. Using in situ heating inside a transmission electron microscope (TEM) while perform-ing electron diffraction, we show that both routes lead to stoichiometrically-controlled formation of PtxSi (x = 1, 2, 3) thin films with high phase selectivity, revealing the crystal structure and formation sequence for each phase. The PtxSi formation process from sequentially-deposited layers of platinum (Pt) and amorphous silicon (a-Si) significantly differs from the Pt/single-crystal silicon (sc-Si) case, allowing the formation of Pt3Si thin films for the first time.
Solid-state reactions to form metal silicides (MexSi) have been widely studied since the early 1980s, and were later used for Ohmic contacts, Schottky barrier contacts, gate electrodes, local interconnects, and diffusion barriers in the microelectronics industry.1‒5 Recently, MexSi have be-come attractive as thermoelectric materials due to their metal-like electrical properties combined with semicon-ductor-like thermal transport.6‒9 Their mechanical robust-ness and thermal stability makes them promising for high temperature engines,1 and combined with their high elec-trical conductivity renders them of interest as next-generation contact materials for nanoelectromechanical (NEM) switches.10‒12 Me
xSi are also considered as alternative plasmonic materials,13 as well as advanced materials for lithium-ion batteries.14 One dimensional transition metal silicides have been studied for their exotic properties such as room temperature ferromagnetism and field emission.15‒17 However, most investigations and applications rely on equilibrium MexSi phases and do not attempt to control the preceding solid-state diffusion reactions that lead to MexSi formation to form specific silicide stoichiometries with de-sired properties.18
Tailoring the physico-chemical properties of MexSi through the precise control of their stoichiometry and crys-tal structure would allow the design of materials suitable for specific applications. Our previous work has shown that the stoichiometry of platinum silicide (PtxSi) films great-ly influences their electrical conductivity: Pt-rich silicides exhibit metallic-like conductivity, while Si-rich silicides are more resistive.10,11 Additionally, the nanoscale adhesion of
these films to Pt tips decreases from Pt-rich to Si-rich films. To ensure precise stoichiometric control, it is neces-sary to understand the synthesis mechanism at the atomic scale and the influence of initial precursor concentration in the ensuing chemical transformation. In situ TEM experi-ments have opened up new frontiers for gaining such un-derstanding.19‒23 Here, we use in situ TEM to introduce two novel routes to precisely control the stoichiometry of thin MexSi films, using PtxSi as a model system. In the first, source-limited solid-state diffusion, precise control of the precursor thin film layer thicknesses predetermines the achievable silicide stoichiometry via annealing. In the se-cond, kinetically-limited solid-state diffusion, a precisely controlled time-temperature regime obtains the desired silicide stoichiometry and phase.
An in situ heating TEM sample holder (Gatan Inc., Pleasanton, CA) was used to anneal the samples in the TEM while continuously recording the electron diffraction pattern (Supporting Information Figure S1), which allowed determination of the crystal structure and formation se-quence of the different PtxSi phases. All samples were sub-jected to similar annealing treatments that included a 10 min hold at 500 ¡C followed by a 10 min hold at 600 ¡C.
The Pt and a-Si films were sputter deposited in a Den-ton Vacuum Explorer 14 sputterer (DenDen-ton Vacuum Inc, Moorestown, NJ) with a purity of 99.99 % for both films. Pt was deposited in DC mode at 450 W and a-Si in AC mode at 230 W. The Pt nanoparticles were produced by coating an a-Si film with approx. 10 nm of Pt, which does not wet the surface completely, forming nanoparticles in-stead of a continuous film.
An in situ heating TEM sample holder (Gatan Inc., Pleasanton, CA) was used to form PtxSi inside the TEM. The heating holder is equipped with a thermocouple sensi-tive to ± 1 ¡C. All source-limited solid-state diffusion sam-ples (Figure 1 and Figure 2) were subject to a similar an-nealing treatment which included the heating up to 500 ¡C (heating rate: 30 ¡C/min) and holding at 500 ¡C for 10 min. This was followed by heating up to 600 ¡C (heating rate: 30 ¡C/min), holding at 600 ¡C for 10 min and rapid cooling to 50 ¡C (cooling rate: 85 ¡C/min). The kinetically-limited solid-state diffusion sample was heated up with a heating rate of 30 ¡C/min until 200 ¡C and rapidly quenched to conserve the Pt3Si phase. Subsequently, the sample was heated up to 300 ¡C (heating rate: 30 ¡C/min) to form Pt2Si followed by rapid quenching. Finally, the sample was heated up to 500 ¡C (heating rate: 30 ¡C/min) to form PtSi and subsequently cooled down.
All TEM experiments were performed using a JEOL 2100 thermionic emission source TEM (JEOL Ltd., Tokyo, Japan). An accelerating voltage of 200 kV was used with a beam current of 106 µA resulting in a current density of 275 pA/cm2.
The chemistry of the near-surface region was investigat-ed by XPS using a customizinvestigat-ed XPS spectrometer (VG Scienta AB, Uppsala, Sweden)24. XPS analyses were per-formed using a monochromatic Al K
α source (photon
ener-gy: 1486.6 eV). The residual pressure in the analysis chamber was constantly less than 1 10-8 Torr. The spec-trometer was calibrated according to ISO 15472:2001 with an accuracy of ± 0.05 eV. Survey and high-resolution spectra were acquired in constant-analyzer-energy mode with the pass energies of 200 eV and 100 eV, respectively. The full width at half-maximum (FWHM) of the peak-height for the high-resolution Ag 3d5/2 signal of a sputter-cleaned Ag sample was 0.57 eV. The spectra were processed using CasaXPS software (v.2.3.16, Case Software Ltd., Wilmslow, Cheshire, U.K.). Background subtraction was performed using the Shirley-Sherwood method. The
quan-titative evaluation of XPS data, as described in 25, was based on integrated intensity using a first-principles model and applying Powell's equation. The inelastic mean free path was calculated using the TPP-2M formula.26 Curve synthesis for the Pt 4f peaks was performed constraining the integrated intensity ratio of these two signals to 3:4 and their energy separation to 3.33 eV. The reference en-ergies for Pt 4f7/2 peaks are 71.05 eV, 71.55 eV, 72.18 eV, and 72.75 eV for Pt, Pt3Si, Pt2Si, and PtSi respectively.
xSi formation. a, Electron diffraction pattern of as-deposited Pt and Pt3Si, Pt2Si, and PtSi films
pro-duced using source-limited solid-state diffusion. Grey slices indicate diffraction ring positions according to the theoretical crystal structure shown schematically for each phase. b, Schematic of the source-limited solid-state diffusion process which utilizes pre-cise control of the Pt and a-Si precursor film thicknesses to predetermine the desired Pt
xSi phase. c, High-resolution XPS spectra
of the Pt4f peaks for as-deposited Pt and resulting PtxSi formed on TEM grids using source-limited solid-state diffusion. PtSi
sam-ple (Pt:a-Si=1:3): quantitative analysis indicates formation of 92% of PtSi. Pt2Si sample (Pt:a-Si=1:1): quantitative analysis indicates
formation of 70% Pt
2Si. Pt3Si sample (Pt:a-Si=2:1): quantitative analysis indicates formation of 74% Pt3Si. Pt sample: quantitative
analysis indicates the presence of pure metallic Pt.
The annealed grids were characterized using high-resolution angle-resolved X-ray photoelectron spectrosco-py (XPS) to determine the stoichiometry of the films(Figure 1c).24 In the high-resolution XPS spectrum of as-deposited Pt ("Pt Sample"), the Pt4f7/2 peak position (71.05±0.05 eV) and lineshape are characteristic of metallic platinum, thus confirming the TEM diffraction pattern displayed in Figure 1a (top-right quadrant). The high-resolution XPS spectrum of the annealed Pt:a-Si=2:1 sample ("Pt3Si Sample") in Figure 1c shows a peak shift assigned to Pt3Si, consistent with the diffraction behavior in Figure 1a (bottom-right quadrant). Quantitative analysis (Figure 1c, insets) deter-mined that this sample consists of 74% Pt3Si and 26% metallic Pt. Figure 1c also shows the high-resolution XPS spectra of the annealed Pt:a-Si=1:1 sample ("Pt2Si Sam-ple"). Quantitative XPS analysis showed that this sample
consists of 70% Pt2Si phase, while the remaining 30% are a mixture between metallic Pt, Pt3Si and PtSi (7% Pt, 14% Pt3Si, 9% PtSi). The high-resolution XPS spectra of the annealed Pt:a-Si=1:3 sample ("PtSi Sample") is displayed in Figure 1c. This sample is composed of 92% PtSi phase (remainder: 2% Pt, 1% Pt3Si, 5% Pt2Si), which matches well with the PtSi diffraction pattern in Figure 1a (left-top quadrant). The quantitative XPS analysis confirmed the PtxSi stoichiometries determined using in situ TEM electron diffraction. The overall results confirm that the stoichiome-try of PtxSi thin films can be precisely tuned using
2. Kinetically-limited Pt
xSi formation. a, Electron diffraction pattern of as-deposited Pt and Pt3Si, Pt2Si, and PtSi films
pro-duced using kinetically-limited solid-state diffusion. Grey slices indicate diffraction ring positions according to the theoretical crystal structure shown schematically for each phase. b, Schematic of the kinetically-limited solid-state diffusion process which utilizes precise control of the temperature-time regime to obtain the desired Pt
xSi phase. c, High-resolution XPS spectra of the Pt4f peaks
for as-deposited Pt and resulting PtxSi formed on TEM grids using kinetically-limited solid-state diffusion. PtSi sample (Pt:a-Si=1:3):
quantitative analysis indicates formation of 91% of PtSi. Pt2Si sample (Pt:a-Si=1:1): quantitative analysis indicates formation of
2Si. Pt3Si sample (Pt:a-Si=2:1): quantitative analysis indicates formation of 88% Pt3Si. Pt sample: quantitative analysis
indi-cates the presence of pure metallic Pt.
-Samples with Pt:a-Si thickness ratio of 1:3 were pro-duced to test if precise control of the temperature-time regime during silicidation can be used to tune the PtxSi stoichiometry (i.e. kinetically-limited solid-state diffusion). This Pt:a-Si thickness ratio will ultimately lead to PtSi for-mation, while passing the Pt3Si and Pt2Si stoichiometries (as seen in Figure 1b). Figure 2 summarizes the results. Figure 2a shows SAD electron diffraction images recorded at room temperature and after the annealing process has been halted at specific temperatures to produce highly selective PtxSi phases. The as-deposited sample, which exhibited a Pt electron diffraction pattern (top-tight quad-rant, Figure 2a), was heated up to 200 ¡C to form Pt3Si and then quickly cooled down to retain this phase at room temperature (bottom-right quadrant). The Pt3Si film was subsequently heated up to 300 ¡C to form Pt2Si and
. Comparison of diffraction pattern intensity distributions obtained from the kinetically-limited and source-limited solid-state diffusion samples. Peak locations and intensity ratios are similar for both methods and indicate that the two methods pro-duce similar Pt
xSi compositions. The theoretical peak positions of the four strongest peaks are indicated by the downward arrows. The annealed TEM grid was characterized using XPS to
determine the stoichiometry of the PtxSi phases formed (Figure 2c). The results presented indicate a similar phase selectivity for kinetically-limited diffusion (88% Pt3Si, 72 % Pt2Si, 91% PtSi) and for the source-limited case (74% Pt3Si, 70% Pt2Si, 92% PtSi). Comparison of the kinetically-limited diffraction patterns (Figure 2a) with those from the source-limited experiments (Figure 1a) show that the peak posi-tions and intensity ratios are similar (Figure 3), which con-firms the similar composition of the PtxSi phases for kinet-ically-limited and source-limited experiments measured using XPS. Figure 2a also shows that all phases formed exhibit minimal grain growth. Dark-field TEM results also indicated that the formed PtxSi films are nanocrystalline. Figure 2b summarizes the kinetically-limited PtxSi formation experiments, and shows that the stoichiometry of PtxSi films was precisely tunable by controlling the temperature-time regime during the annealing. The in situ TEM experi-ments presented in Figure 2 prove that kinetically-controlled solid-state diffusion is a highly effective way to tune the PtxSi stoichiometry.
Both source-limited and kinetically-limited solid-state dif-fusion experiments (Figure 1, Figure 2) were able to pro-duce highly selective Pt3Si films, which have not been ex-perimentally reported before or observed during Pt/sc-Si experiments. The well-studied Pt/sc-Si system is charac-terized by the specific PtxSi formation sequence of Pt dif-fusing into sc-Si around 250-300 ¡C to form the interme-diate Pt2Si phase. After all Pt is consumed, sc-Si will dif-fuse into Pt2Si at 300-450 ¡C to form the thermodynami-cally stable PtSi phase.27,28 We propose that the amorphous
nature of the a-Si film used in our experiments alters the diffusion behavior compared to sc-Si, which leads to the formation of the Pt3Si phase. The Pt3Si phase is formed due to the fact that in the Pt/a-Si system, a-Si acts initially as the dominant diffusing species (DDS) in contrast to the Pt/sc-Si system where Pt is initially the DDS. The distribu-tion of bonding characteristics of a-Si compared to sc-Si leads to reduced activation energies for a-Si self-diffusion of up to 27% compared to those for sc-Si.29 Thus, a-Si becomes mobile at lower temperatures than sc-Si. In ad-dition to the increased mobility of a-Si, the Pt diffusivity is drastically reduced in a-Si compared to sc-Si. Pt has a diffusion coefficient at 500 ¡C of ~5 10-18 m2/s in a-Si,30 whereas the diffusion coefficient of Pt in sc-Si is ~5 10-16 m2/s,31 which means that Pt diffuses two orders of magni-tude faster in sc-Si than in a-Si. Both the increased a-Si and reduced Pt diffusivity contribute to the a-Si diffusion into Pt and subsequent formation of Pt3Si for the Pt/a-Si system.
4. Determination of the dominant diffusing species (DDS) during Pt
3Si formation. a, The schematic and the TEM image on
the left shows the as-deposited sample: an a-Si film covered by Pt nanoparticles. Annealing will lead to Pt3Si formation. If Pt is the
DDS, then the Pt nanoparticles will completely diffuse into the underlying a-Si layer and the Pt-containing region (high Z contrast) will appear larger in TEM images. If Si is the DDS, then the nanoparticle shape and size will be nearly preserved and no major change of the high Z contrast region will be visible in the TEM. b, TEM images of several Pt nanoparticles before (at 130 ¡C) and after (280 ¡C) Pt3Si formation. The overall shape and size of the Pt and Pt3Si nanoparticles is similar, indicating that Pt3Si formation
occurs through diffusion of a-Si into Pt. The electron diffraction pattern shows that Pt
3Si particles were formed. To demonstrate that a-Si is the diffusing species instead
of Pt and that this leads to Pt3Si formation, we coated a Si3N4-support TEM grid with a-Si and, subsequently, with Pt nanoparticles of ~10 nm diameter (as shown in Figure 4a). Figure 4a shows a schematic and TEM image of the as-deposited sample together with the theoretical path-ways leading to the formation of Pt3Si, i.e., the diffusion of Pt in a-Si or the diffusion of a-Si in Pt. If Pt is the DDS, then the Pt nanoparticles will diffuse into the underlying a -Si layer and a TEM Z-contrast image will show significant broadening of the Pt-containing regions. If, on the other hand, a-Si is the diffusing species as proposed here, then the general shape of the Pt nanoparticles should be con-served during Pt3Si formation as only a small amount of a -Si is diffusing into the nanoparticles. Figure 4b shows an area of the sample with several Pt nanoparticles before (at 130 ¡C) and after (at 280 ¡C) Pt3Si formation. The overall shape and size of the nanoparticles do not undergo any significant changes due to Pt3Si formation. This result con-firms that a-Si is the DDS, and that it diffuses into Pt to form Pt3Si, which means that the occurrence of Pt3Si in a -Si-based silicidation experiments is entirely due to the high diffusivity of a-Si, and that such films are not attainable using sc-Si.
The Pt3Si films resulting from Pt/a-Si annealing have sev-eral advantages over PtSi films that result from Pt/sc-Si. Most notably, Pt3Si possesses similar mechanical
proper-ties as PtSi (~50% greater hardness and modulus com-pared to Pt),10 but with a higher electrical conductivity.10,11 The increased hardness of Pt3Si can also be understood from our source-limited heating experiments where we observe not only grain coarsening but also formation of anti-phase boundaries (APBs) (Supporting Information Figure S2), which are two dimensional defects commonly found in L12 type crystal structures.32-35 These APBs will hinder disloca-tion modisloca-tion and thereby plastic deformadisloca-tion.
stoichi-ometry with significant potential as an electrical conductive and wear-resistive coating.
. Schematics of the experimental procedure and TEM images of the anti-phase boundaries found in Pt3Si can be found in the supporting information. This
material is available free of charge via the Internet at http://pubs.acs.org.
!Laboratoire de Tribologie et Dynamique des Syst•mes, Ecole
Centrale de Lyon, 35 Avenue Guy de Collongue, Ecully, 69134 France.
All authors have given approval to the final version of the manuscript. ¤ These authors contributed equally. The authors declare no competing financial interest.
The authors acknowledge the use of instrumentation from the Nano/Bio Interface Center (NBIC) and the Nanoscale Charac-terization Facility (NCF) at the University of Pennsylvania. Funding from the DMREF program of the National Science Foundation (award number: CMMI-1334241) is acknowl-edged. F.M. acknowledges support from the Marie Curie In-ternational Outgoing Fellowship for Career Development with-in the 7th European Community Framework Program under
contract no. PIOF-GA-2012-328776.
(1) Miglio, L.; d'Heurle, F. Silicides - Fundamentals and
Appli-cations; World Scientific Publishing: Singapore, 2000.
(2) Peter, A. P.; Meersschaut, J.; Richard, O.; Moussa, A.; Steenbergen, J.; Schaekers, M.; Tokei, Z.; Van Elshocht, S.;
Adelmann, C. Chem. Mater. , 27, 245-254.
(3) Tu, K. N.; Thompson, R. D.; Tsaur, B. Y. Applied Physics
Letters , 38, 626-628.
(4) Rhoderick, E. H.; Williams, R. H. Metal-Semiconductor
Contacts, Clarendon Press: Oxford, 1988.
(5) Chen, L. J. JOM , 57, 24-31.
(6) Rowe, D. M. Thermoelectrics Handbook: Macro to Nano,
Taylor & Francis Group: Abingdon, 2006.
(7) Fedoriv, M. I. J. Thermoelectr. , 2, 51-60.
(8) Itoh, T.; Yamada, M. J. Electron. Mater. , 38,
(9) de Boor, J.; Dasgupta, T.; Kolb, H.; Compere, C.; Kelm, K.;
Mueller, E. Acta Mater. , , 68-75.
(10) Streller, F.; Wabiszewski, G. W.; Mangolini, F.; Feng, G.;
Carpick, R. W. Adv. Mater. Interfaces , 1, 1300120.
(11) Streller, F.; Wabiszewski, G. E.; Carpick, R. W. IEEE
Nano-technol. Mag., DOI: 10.11109/MNANO.2014.2373451.
(12) Loh, O. Y.; Espinosa, H. D. Nat. Nanotechnol. , 7,
(13) Naik, G. V.; Shalaev, V. M.; Boltasseva, A. Adv. Mater.
, 25, 3264-3294.
(14) Liu, C; Li, F.; Ma, L.-P.; Cheng, H.-M. Adv. Mater. 0,
(15) Lin, H.-K.; Cheng, H.-A; Lee, C.-Y.; Chiu, H.-T. Chem.
Mater. , 21, 5388-5396.
(16) Li, H.; Wu, J.; Wang, Z. M. Silicon-based Nanomaterials,
Springer: Berlin, 2013.
(17) Higgins, J. M.; Ding, R.; Jin, S. Chem. Mater. 1, 23,
(18) Schmitt, A. L.; Higgins, J. M.; Szczech, J. R.; Jin, S. J.
Mater. Chem. , 20, 223-235.
(19) Chou, Y.-C.; Wu, W.-W.; Cheng, S.-L.; Yoo, B.-Y.;
Myung, N.; Chen, L. J.; Tu, K. N. Nano Lett. , 8,
(20) Liu, X. H.; Wang, J. W.; Huang, S.; Fan, F.; Huang, X.; Liu, Y.; Krylyk, S.; Yoo, J.; Dayeh, S. A.; Davydov, A. V.; Mao, S. C.;
Picraux, T.; Zhang, S.; Li, J.; Zhy, T.; Huang, J. Y. Nat.
Nano-technol. , 7, 749-756.
(21) Lin, Y.-C.; Chen, Y.; Xu, D.; Huang, Y. Nano Lett. ,
(22) Stach, E. A.; Pauzauskie, P. J.; Kuykendall, T.;
Gold-berger, J.; He, R.; Yang, P. Nano Lett. , 3, 867-869.
(23) Nukala, P.; Agarwal, R.; Qian, X.; Jang, M. H.; Dhara, S.;
Kumar, K.; Johnson, A. T. C.; Li, J.; Agarwal, R. Nano Lett.
, 14, 2201-2209.
(24) Mangolini, F.; Ahlund, J.; Wabiszewski, G. E.; Adiga, V. P.; Egberts, P.; Streller, F.; Backlund, K.; Karlsson, P. G.; Wannberg,
B.; Carpick, R. W. Rev. Sci. Instrum. , 83, 093112.
(25) Mangolini, F.; Rossi, A.; Spencer, N. D. J. Phys. Chem. C
, 115, 1339-1354.
(26) Tanuma, S. Surface Analysis by Auger and X-Ray Photoe-lectron Spectroscopy, IM Publications: Charlton, 2003.
(27) Stark, T.; Gruenleitner, H.; Hundhausen, M.; Ley, L. Thin
Solid Films , 358, 73-79.
(28) Poate, J. M.; Tisone, T. C. Appl. Phys. Lett. , 24,
(29) Kobayashi, T.; Koguchi, M.; Iijima, S.; Ohkura, M. J.
Elec-trochem. Soc. , 141, 1365-1369.
(30) Coffa, S.; Poate, J. M.; Jacobson, D. C. Phys. Rev. B
, 45, 8355-8358.
(31) Lerch, W.; Stolwijk, N. A.; Mehrer, H.; Poisson, C.
Semi-cond. Sci. Technol. , 10, 1257-1263.
(32) Tichelaar, F. D.; Schapink, F. W. Philos. Mag. A , 54,
(33) Tichelaar, F. D.; Schapink, F. W. J. Phys. Colloq. ,
(34) Janowski, G. M.; Stafford, G. R. Metall. Trans. A ,
(35) Chou, T. C.; Chou, Y. T. MTS Proceedings , 39,